Comparative study of structures, thermal stabilities and dielectric properties for a ferroelectric MOF [Sr(μ-BDC)(DMF)]∞with its solvent-free framework.
Guo, Ping-Chun; Chu, Zhenyu; Ren, Xiao-Ming; Ning, Wei-Hua; Jin, Wanqin; Dalton transactions (Cambridge, England : 2003) 42 (2013) 6603–6610; doi:10.1039/c3dt32880e

data_7022707
_publ_section_title
;
 Comparative study of structures, thermal stabilities and dielectric
 properties for a ferroelectric MOF [Sr(\m-BDC)(DMF)]\\infty with its
 solvent-free framework.
;
_journal_issue                   18
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              6603
_journal_page_last               6610
_journal_paper_doi               10.1039/c3dt32880e
_journal_volume                  42
_journal_year                    2013
_chemical_formula_sum            'C11 H11 N O5 Sr'
_chemical_formula_weight         324.83
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           144
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'P 31'
_symmetry_space_group_name_H-M   'P 31'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   10.6123(2)
_cell_length_b                   10.6123(2)
_cell_length_c                   9.8289(2)
_cell_measurement_reflns_used    3665
_cell_measurement_temperature    243(2)
_cell_measurement_theta_max      62.4353
_cell_measurement_theta_min      4.4948
_cell_volume                     958.64(3)
_computing_cell_refinement
;
 CrysAlisPro, Oxford Diffraction Ltd.,
 Version 1.171.33.46 (release 27-08-2009 CrysAlis171 .NET)
 (compiled Aug 27 2009,17:19:36)
;
_computing_data_collection
;
 CrysAlisPro, Oxford Diffraction Ltd.,
 Version 1.171.33.46 (release 27-08-2009 CrysAlis171 .NET)
 (compiled Aug 27 2009,17:19:36)
;
_computing_data_reduction
;
 CrysAlisPro, Oxford Diffraction Ltd.,
 Version 1.171.33.46 (release 27-08-2009 CrysAlis171 .NET)
 (compiled Aug 27 2009,17:19:36)
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      243(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measurement_device_type  'Xcalibur, Sapphire3, Gemini ultra'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0177
_diffrn_reflns_av_sigmaI/netI    0.0158
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            3656
_diffrn_reflns_theta_full        62.53
_diffrn_reflns_theta_max         62.53
_diffrn_reflns_theta_min         6.59
_exptl_absorpt_coefficient_mu    6.005
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.57412
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.688
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             486
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.524
_refine_diff_density_min         -0.391
_refine_diff_density_rms         0.061
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.037(19)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.115
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     165
_refine_ls_number_reflns         1485
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.114
_refine_ls_R_factor_all          0.0204
_refine_ls_R_factor_gt           0.0204
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0348P)^2^+0.6542P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0553
_refine_ls_wR_factor_ref         0.0554
_reflns_number_gt                1481
_reflns_number_total             1485
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3dt32880e.cif
_cod_data_source_block           243K
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      P3(1)
_cod_database_code               7022707